##############################################################################
#                                                                            #
# This CIF contains the data in a paper accepted for publication in Acta     #
# Crystallographica Section B. It has been peer reviewed under the auspices  #
# of the IUCr Commission on Journals.                                        #
#                                                                            #
# Full details of the Crystallographic Information File format               #
# are given in the paper "The Crystallographic Information File (CIF):       #
# a New Standard Archive File for Crystallography" by S. R. Hall, F. H.      #
# Allen and I. D. Brown [Acta Cryst. (1991), A47, 655-685].                  #
#                                                                            #
# The current version of the core CIF dictionary may be obtained from        #
# ftp://ftp.iucr.org/pub/cif_core.dic. The current version number is 2.1.    #
#                                                                            #
# Software is freely available for graphical display of the structure(s) in  #
# this CIF.  For information consult the CIF home page http://www.iucr.org/  #
# cif/home.html                                                              #
#                                                                            #
#           Copyright International Union of Crystallography                 #
#                                                                            #
##############################################################################

data_global
_audit_creation_method     'Jana2000 Version : 22/12/2005'
_journal_date_recd_electronic     2007-01-30
_journal_date_accepted     2007-05-29
_journal_name_full     'Acta Crystallographica, Section B'
_journal_year     2007
_journal_volume     63
_journal_issue      4
_journal_page_first     545
_journal_page_last     550
_journal_paper_category     FA
_journal_coeditor_code     CK5025
_publ_contact_author_name     ?
_publ_contact_author_address
; ?
;
_publ_contact_author_email     ?
_publ_contact_author_fax     ?
_publ_contact_author_phone     ?
_publ_section_title
; ?
;
_publ_section_title_footnote
; ?
;
loop_
    _publ_author_name
    _publ_author_footnote
    _publ_author_address
    ?
; ?      # footnote
;
; ?      # address
;
_publ_section_synopsis
; ?
;
data_1
_chemical_name_systematic
; ?
;
_chemical_name_common     ?
_chemical_formula_moiety     ?
_chemical_formula_sum     'Ge1 Na1 O5 Ta1'
_chemical_formula_structural     ?
_chemical_formula_analytical     ?
_chemical_formula_iupac     ?
_chemical_formula_weight     356.5
_chemical_melting_point     ?
_symmetry_cell_setting     monoclinic
_symmetry_space_group_name_H-M     'P 1 21/c 1'
_symmetry_space_group_name_Hall     '-P 2ybc'
loop_
    _symmetry_equiv_pos_site_id
    _symmetry_equiv_pos_as_xyz
    1 x,y,z
    2 -x,1/2+y,1/2-z
    3 -x,-y,-z
    4 x,1/2-y,1/2+z
_cell_length_a     6.8380(10)
_cell_length_b     8.9300(10)
_cell_length_c     7.4140(10)
_cell_angle_alpha     90
_cell_angle_beta     114.800(6)
_cell_angle_gamma     90
_cell_volume     411.00(10)
_cell_formula_units_Z     4
_cell_measurement_reflns_used     ?
_cell_measurement_theta_min     ?
_cell_measurement_theta_max     ?
_cell_measurement_temperature     98
_cell_special_details
; ?
;
_exptl_crystal_description     Tabular
_exptl_crystal_colour     'colourless'
_exptl_crystal_size_max     0.1
_exptl_crystal_size_mid     0.09
_exptl_crystal_size_min     0.045
_exptl_crystal_size_rad     ?
_exptl_crystal_density_diffrn     5.7603
_exptl_crystal_density_meas     ?
_exptl_crystal_density_method     ?
_exptl_crystal_F_000     624
_exptl_absorpt_coefficient_mu     6.97
_exptl_absorpt_correction_type     None
_exptl_absorpt_process_details     ?
_exptl_absorpt_correction_T_min     ?
_exptl_absorpt_correction_T_max     ?
_exptl_special_details     ?
_diffrn_ambient_temperature     98
_diffrn_radiation_type     'synchrotron'
_diffrn_radiation_wavelength     0.39184
_diffrn_radiation_source     ?
_diffrn_radiation_monochromator     ?
_diffrn_measurement_device_type     'beamline F1 at Hasylab'
_diffrn_measurement_method     'φ-scan'
_diffrn_detector_area_resol_mean     ?
_diffrn_reflns_number     95016
_diffrn_reflns_av_R_equivalents     0.0438
_diffrn_reflns_av_sigmaI/netI     0.0349
_diffrn_reflns_theta_min     1.81
_diffrn_reflns_theta_max     45.87
_diffrn_reflns_theta_full     45.87
_diffrn_measured_fraction_theta_max     ?
_diffrn_measured_fraction_theta_full     0.97
_diffrn_reflns_limit_h_min     -25
_diffrn_reflns_limit_h_max     25
_diffrn_reflns_limit_k_min     -32
_diffrn_reflns_limit_k_max     27
_diffrn_reflns_limit_l_min     -27
_diffrn_reflns_limit_l_max     23
_diffrn_reflns_reduction_process     ?
_refine_special_details
; ?
;
_reflns_number_total     20505
_reflns_number_gt     17954
_reflns_threshold_expression     'I>3σ(I)'
_refine_ls_structure_factor_coef     Fsqd
_refine_ls_R_factor_all     0.0273
_refine_ls_R_factor_gt     0.0230
_refine_ls_wR_factor_gt     0.0692
_refine_ls_wR_factor_ref     0.0728
_refine_ls_goodness_of_fit_ref     1.06
_refine_ls_restrained_S_all     ?
_refine_ls_number_reflns     20505
_refine_ls_number_parameters     74
_refine_ls_number_restraints     ?
_refine_ls_number_constraints     ?
_refine_ls_hydrogen_treatment     ?
_refine_ls_weighting_scheme     sigma
_refine_ls_weighting_details     'w=1/(σ²(I)+0.0016I²)'
_refine_ls_shift/su_max     0.0124
_refine_ls_shift/su_mean     0.0004
_refine_diff_density_max     2.95
_refine_diff_density_min     -4.68
_refine_ls_extinction_method
                        'B-C type 1 Gaussian isotropic (Becker & Coppens, 1974)'
_refine_ls_extinction_coef     0.00345(16)
loop_
    _atom_type_symbol
    _atom_type_scat_dispersion_real
    _atom_type_scat_dispersion_imag
    _atom_type_scat_source
    Ge 0.275 0.650 'International Tables Vol C Tables  4.2.6.8 and 6.1.1.4'
    Na 0.009 0.007 'International Tables Vol C Tables  4.2.6.8 and 6.1.1.4'
    O 0.002 0.002 'International Tables Vol C Tables  4.2.6.8 and 6.1.1.4'
    Ta -0.553 2.507 'International Tables Vol C Tables  4.2.6.8 and 6.1.1.4'
_computing_data_collection     ?
_computing_cell_refinement     ?
_computing_data_reduction     ?
_computing_structure_solution     ?
_computing_structure_refinement     '(Jana2000; Petricek and Dusek, 2000)'
_computing_molecular_graphics     ?
_computing_publication_material     '(Jana2000; Petricek and Dusek, 2000)'
loop_
    _atom_site_type_symbol
    _atom_site_label
    _atom_site_fract_x
    _atom_site_fract_y
    _atom_site_fract_z
    _atom_site_U_iso_or_equiv
    _atom_site_adp_type
    _atom_site_calc_flag
    _atom_site_refinement_flags
    _atom_site_occupancy
    _atom_site_disorder_assembly
    _atom_site_disorder_group
    Na Na 0.24827(4) 0.92207(6) 0.24235(5) 0.01108(10) Uani d . 1 . .
    Ta Ta 0.748245(2) 0.752060(2) 0.504007(3) 0.003180(5) Uani d . 1 . .
    Ge Ge 0.249340(6) 0.567282(8) 0.249414(6) 0.003072(8) Uani d . 1 . .
    O O1 0.25058(5) 0.18307(5) 0.24884(4) 0.00508(5) Uani d . 1 . .
    O O2 0.44387(6) 0.68888(4) 0.41119(6) 0.00602(5) Uani d . 1 . .
    O O3 0.94724(6) 0.18710(4) 0.41330(6) 0.00594(5) Uani d . 1 . .
    O O4 0.35039(6) 0.45542(4) 0.11373(6) 0.00544(5) Uani d . 1 . .
    O O5 0.84765(6) 0.95470(4) 0.11214(6) 0.00540(5) Uani d . 1 . .
loop_
    _atom_site_aniso_label
    _atom_site_aniso_U_11
    _atom_site_aniso_U_22
    _atom_site_aniso_U_33
    _atom_site_aniso_U_12
    _atom_site_aniso_U_13
    _atom_site_aniso_U_23
    _atom_site_aniso_type_symbol
    Na 0.00875(12) 0.00526(9) 0.01730(19) -0.00006(5) 0.00358(12) -0.00022(7) Na
    Ta 0.002967(6) 0.003137(6) 0.003265(7) -0.000264(2) 0.001138(5) 0.000239(2)
                                                                              Ta
    Ge 0.002880(10)
                  0.002980(10)
                             0.003230(10)
                                        0.000007(5) 0.001150(8) -0.000005(6) Ge
    O1 0.00648(8) 0.00553(8) 0.00360(6) 0.00003(4) 0.00248(6) 0.00003(5) O
    O2 0.00439(7) 0.00633(8) 0.00681(8) -0.00152(6) 0.00183(6) -0.00164(7) O
    O3 0.00457(7) 0.00619(8) 0.00663(8) -0.00150(6) 0.00192(6) -0.00151(7) O
    O4 0.00622(7) 0.00451(7) 0.00654(8) -0.00052(5) 0.00360(6) -0.00135(6) O
    O5 0.00621(7) 0.00440(6) 0.00646(8) -0.00048(5) 0.00351(6) -0.00122(6) O
loop_
    _geom_bond_atom_site_label_1
    _geom_bond_atom_site_label_2
    _geom_bond_site_symmetry_1
    _geom_bond_site_symmetry_2
    _geom_bond_distance
    _geom_bond_publ_flag
    Na O1 . 1_565 2.3312(7) yes
    Na O2 . . 2.5075(6) yes
    Na O3 . 2_655 2.4956(6) yes
    Na O4 . 2_655 2.5104(5) yes
    Na O4 . 4_565 2.7664(6) yes
    Na O5 . 1_455 2.5106(5) yes
    Na O5 . 3_675 2.6651(6) yes
    Ta O1 . 3_666 1.9186(3) yes
    Ta O1 . 2_655 1.9765(3) yes
    Ta O2 . . 1.9805(4) yes
    Ta O3 . 3_766 1.9839(4) yes
    Ta O4 . 2_655 2.0052(4) yes
    Ta O5 . 4_565 2.0141(4) yes
    Ge O2 . . 1.7461(4) yes
    Ge O3 . 2_655 1.7455(4) yes
    Ge O4 . . 1.7523(5) yes
    Ge O5 . 2_645 1.7536(5) yes
    O1 O2 . 3_666 2.7582(4) yes
    O1 O2 . 2_645 2.8027(6) yes
    O1 O3 . 1_455 2.8129(6) yes
    O1 O3 . 4_454 2.7398(4) yes
    O1 O4 . . 2.8210(6) yes
    O1 O4 . 4_555 2.7866(5) yes
    O1 O5 . 3_665 2.7604(5) yes
    O1 O5 . 2_645 2.8245(6) yes
    O2 O3 . 2_655 2.7465(4) yes
    O2 O4 . . 2.9045(6) yes
    O2 O4 . 2_655 2.8101(6) yes
    O2 O5 . 2_645 2.8438(6) yes
    O2 O5 . 4_565 2.8348(5) yes
    O3 O4 . 2_645 2.8496(6) yes
    O3 O4 . 4_655 2.8268(5) yes
    O3 O5 . 1_545 2.9121(6) yes
    O3 O5 . 2_745 2.8170(6) yes
    O4 O5 . 2_645 2.8763(7) yes
loop_
    _geom_angle_atom_site_label_1
    _geom_angle_atom_site_label_2
    _geom_angle_atom_site_label_3
    _geom_angle_site_symmetry_1
    _geom_angle_site_symmetry_2
    _geom_angle_site_symmetry_3
    _geom_angle
    _geom_angle_publ_flag
    O1 Na O2 1_565 . . 145.328(16) yes
    O1 Na O3 1_565 . 2_655 147.984(16) yes
    O1 Na O4 1_565 . 2_655 82.870(17) yes
    O1 Na O4 1_565 . 4_565 65.630(16) yes
    O1 Na O5 1_565 . 1_455 83.612(18) yes
    O1 Na O5 1_565 . 3_675 66.688(17) yes
    O2 Na O3 . . 2_655 66.590(18) yes
    O2 Na O4 . . 2_655 68.114(15) yes
    O2 Na O4 . . 4_565 88.420(17) yes
    O2 Na O5 . . 1_455 123.77(2) yes
    O2 Na O5 . . 3_675 133.97(2) yes
    O3 Na O4 2_655 . 2_655 125.06(2) yes
    O3 Na O4 2_655 . 4_565 130.95(2) yes
    O3 Na O5 2_655 . 1_455 68.486(15) yes
    O3 Na O5 2_655 . 3_675 91.641(17) yes
    O4 Na O4 2_655 . 4_565 75.846(16) yes
    O4 Na O5 2_655 . 1_455 166.33(3) yes
    O4 Na O5 2_655 . 3_675 98.23(2) yes
    O4 Na O4 4_565 . 2_655 75.846(16) yes
    O4 Na O5 4_565 . 1_455 96.660(19) yes
    O4 Na O5 4_565 . 3_675 132.32(2) yes
    O5 Na O5 1_455 . 3_675 78.193(16) yes
    O5 Na O5 3_675 . 1_455 78.193(16) yes
    O1 Ta O1 3_666 . 2_655 179.273(16) yes
    O1 Ta O2 3_666 . . 90.036(16) yes
    O1 Ta O3 3_666 . 3_766 92.224(16) yes
    O1 Ta O4 3_666 . 2_655 90.470(18) yes
    O1 Ta O5 3_666 . 4_565 91.782(18) yes
    O1 Ta O1 2_655 . 3_666 179.272(16) yes
    O1 Ta O2 2_655 . . 90.196(16) yes
    O1 Ta O3 2_655 . 3_766 87.545(16) yes
    O1 Ta O4 2_655 . 2_655 90.220(18) yes
    O1 Ta O5 2_655 . 4_565 87.527(18) yes
    O2 Ta O3 . . 3_766 177.739(19) yes
    O2 Ta O4 . . 2_655 89.665(16) yes
    O2 Ta O5 . . 4_565 90.411(16) yes
    O3 Ta O4 3_766 . 2_655 90.246(16) yes
    O3 Ta O5 3_766 . 4_565 89.589(16) yes
    O4 Ta O5 2_655 . 4_565 177.747(19) yes
    O2 Ge O3 . . 2_655 103.739(17) yes
    O2 Ge O4 . . . 112.25(2) yes
    O2 Ge O5 . . 2_645 108.703(19) yes
    O3 Ge O4 2_655 . . 109.12(2) yes
    O3 Ge O5 2_655 . 2_645 112.66(2) yes
    O4 Ge O5 . . 2_645 110.26(2) yes
    Na O1 Ta 1_545 . 3_666 108.59(2) yes
    Na O1 Ta 1_545 . 2_645 107.142(19) yes
    Na O1 O2 1_545 . 3_666 115.425(16) yes
    Na O1 O2 1_545 . 2_645 90.548(18) yes
    Na O1 O3 1_545 . 1_455 91.254(18) yes
    Na O1 O3 1_545 . 4_454 114.101(16) yes
    Na O1 O4 1_545 . . 148.78(2) yes
    Na O1 O4 1_545 . 4_555 64.728(16) yes
    Na O1 O5 1_545 . 3_665 62.456(16) yes
    Na O1 O5 1_545 . 2_645 149.95(2) yes
    Ta O1 Ta 3_666 . 2_645 144.26(3) yes
    Ta O1 O2 3_666 . 3_666 45.891(12) yes
    Ta O1 O2 3_666 . 2_645 133.909(16) yes
    Ta O1 O3 3_666 . 1_455 44.811(11) yes
    Ta O1 O3 3_666 . 4_454 115.96(2) yes
    Ta O1 O4 3_666 . . 100.028(19) yes
    Ta O1 O4 3_666 . 4_555 46.020(11) yes
    Ta O1 O5 3_666 . 3_665 164.24(2) yes
    Ta O1 O5 3_666 . 2_645 45.459(13) yes
    Ta O1 Ta 2_645 . 3_666 144.26(3) yes
    Ta O1 O2 2_645 . 3_666 115.762(19) yes
    Ta O1 O2 2_645 . 2_645 44.960(10) yes
    Ta O1 O3 2_645 . 1_455 134.770(15) yes
    Ta O1 O3 2_645 . 4_454 46.340(12) yes
    Ta O1 O4 2_645 . . 45.302(12) yes
    Ta O1 O4 2_645 . 4_555 164.23(2) yes
    Ta O1 O5 2_645 . 3_665 46.801(11) yes
    Ta O1 O5 2_645 . 2_645 100.056(19) yes
    O2 O1 O2 3_666 . 2_645 88.036(15) yes
    O2 O1 O3 3_666 . 1_455 90.701(16) yes
    O2 O1 O3 3_666 . 4_454 130.47(2) yes
    O2 O1 O4 3_666 . . 76.333(15) yes
    O2 O1 O4 3_666 . 4_555 60.899(13) yes
    O2 O1 O5 3_666 . 3_665 148.624(19) yes
    O2 O1 O5 3_666 . 2_645 61.018(13) yes
    O2 O1 O2 2_645 . 3_666 88.036(15) yes
    O2 O1 O3 2_645 . 1_455 178.12(2) yes
    O2 O1 O3 2_645 . 4_454 91.300(16) yes
    O2 O1 O4 2_645 . . 59.958(15) yes
    O2 O1 O4 2_645 . 4_555 119.781(16) yes
    O2 O1 O5 2_645 . 3_665 61.265(14) yes
    O2 O1 O5 2_645 . 2_645 118.176(19) yes
    O3 O1 O3 1_455 . 4_454 88.458(16) yes
    O3 O1 O4 1_455 . . 118.369(19) yes
    O3 O1 O4 1_455 . 4_555 60.639(14) yes
    O3 O1 O5 1_455 . 3_665 120.145(16) yes
    O3 O1 O5 1_455 . 2_645 59.959(15) yes
    O3 O1 O3 4_454 . 1_455 88.458(16) yes
    O3 O1 O4 4_454 . . 61.088(14) yes
    O3 O1 O4 4_454 . 4_555 148.56(2) yes
    O3 O1 O5 4_454 . 3_665 61.615(13) yes
    O3 O1 O5 4_454 . 2_645 76.265(15) yes
    O4 O1 O4 . . 4_555 136.900(16) yes
    O4 O1 O5 . . 3_665 92.104(16) yes
    O4 O1 O5 . . 2_645 61.260(17) yes
    O4 O1 O4 4_555 . . 136.900(16) yes
    O4 O1 O5 4_555 . 3_665 127.18(2) yes
    O4 O1 O5 4_555 . 2_645 91.478(16) yes
    O5 O1 O5 3_665 . 2_645 137.574(16) yes
    O5 O1 O5 2_645 . 3_665 137.574(16) yes
    Na O2 Ta . . . 101.516(18) yes
    Na O2 Ge . . . 94.611(16) yes
    Na O2 O1 . . 3_666 98.794(18) yes
    Na O2 O1 . . 2_655 98.06(2) yes
    Na O2 O3 . . 2_655 56.496(14) yes
    Na O2 O4 . . . 108.397(17) yes
    Na O2 O4 . . 2_655 55.991(14) yes
    Na O2 O5 . . 2_645 111.519(16) yes
    Na O2 O5 . . 4_565 146.72(2) yes
    Ta O2 Ge . . . 143.38(3) yes
    Ta O2 O1 . . 3_666 44.073(10) yes
    Ta O2 O1 . . 2_655 44.844(12) yes
    Ta O2 O3 . . 2_655 143.26(2) yes
    Ta O2 O4 . . . 109.44(2) yes
    Ta O2 O4 . . 2_655 45.525(11) yes
    Ta O2 O5 . . 2_645 146.961(19) yes
    Ta O2 O5 . . 4_565 45.274(11) yes
    Ge O2 O1 . . 3_666 162.24(2) yes
    Ge O2 O1 . . 2_655 100.72(2) yes
    Ge O2 O3 . . 2_655 38.123(11) yes
    Ge O2 O4 . . . 33.944(13) yes
    Ge O2 O4 . . 2_655 137.71(2) yes
    Ge O2 O5 . . 2_645 35.737(13) yes
    Ge O2 O5 . . 4_565 111.910(19) yes
    O1 O2 O1 3_666 . 2_655 88.916(15) yes
    O1 O2 O3 3_666 . 2_655 152.74(2) yes
    O1 O2 O4 3_666 . . 146.358(19) yes
    O1 O2 O4 3_666 . 2_655 60.048(14) yes
    O1 O2 O5 3_666 . 2_645 127.11(2) yes
    O1 O2 O5 3_666 . 4_565 60.645(13) yes
    O1 O2 O1 2_655 . 3_666 88.916(15) yes
    O1 O2 O3 2_655 . 2_655 104.713(19) yes
    O1 O2 O4 2_655 . . 68.345(16) yes
    O1 O2 O4 2_655 . 2_655 60.343(16) yes
    O1 O2 O5 2_655 . 2_645 126.06(2) yes
    O1 O2 O5 2_655 . 4_565 58.631(14) yes
    O3 O2 O4 2_655 . . 60.489(14) yes
    O3 O2 O4 2_655 . 2_655 106.124(17) yes
    O3 O2 O5 2_655 . 2_645 62.759(14) yes
    O3 O2 O5 2_655 . 4_565 146.48(2) yes
    O4 O2 O4 . . 2_655 120.99(2) yes
    O4 O2 O5 . . 2_645 60.039(15) yes
    O4 O2 O5 . . 4_565 85.988(16) yes
    O4 O2 O4 2_655 . . 120.99(2) yes
    O4 O2 O5 2_655 . 2_645 167.507(17) yes
    O4 O2 O5 2_655 . 4_565 90.777(15) yes
    O5 O2 O5 2_645 . 4_565 101.695(16) yes
    O5 O2 O5 4_565 . 2_645 101.695(16) yes
    Na O3 Ta 2_645 . 3_766 101.647(19) yes
    Na O3 Ge 2_645 . 2_645 95.044(16) yes
    Na O3 O1 2_645 . 1_655 99.19(2) yes
    Na O3 O1 2_645 . 4_655 96.822(18) yes
    Na O3 O2 2_645 . 2_645 56.914(14) yes
    Na O3 O4 2_645 . 2_645 110.465(17) yes
    Na O3 O4 2_645 . 4_655 146.80(2) yes
    Na O3 O5 2_645 . 1_545 109.695(17) yes
    Na O3 O5 2_645 . 2_745 56.010(14) yes
    Ta O3 Ge 3_766 . 2_645 141.78(3) yes
    Ta O3 O1 3_766 . 1_655 42.965(11) yes
    Ta O3 O1 3_766 . 4_655 46.115(11) yes
    Ta O3 O2 3_766 . 2_645 141.19(2) yes
    Ta O3 O4 3_766 . 2_645 147.848(19) yes
    Ta O3 O4 3_766 . 4_655 45.181(11) yes
    Ta O3 O5 3_766 . 1_545 108.04(2) yes
    Ta O3 O5 3_766 . 2_745 45.641(11) yes
    Ge O3 O1 2_645 . 1_655 100.76(2) yes
    Ge O3 O1 2_645 . 4_655 163.18(3) yes
    Ge O3 O2 2_645 . 2_645 38.138(11) yes
    Ge O3 O4 2_645 . 2_645 35.521(13) yes
    Ge O3 O4 2_645 . 4_655 112.696(19) yes
    Ge O3 O5 2_645 . 1_545 33.758(13) yes
    Ge O3 O5 2_645 . 2_745 137.26(2) yes
    O1 O3 O1 1_655 . 4_655 89.077(15) yes
    O1 O3 O2 1_655 . 2_645 104.155(19) yes
    O1 O3 O4 1_655 . 2_645 126.51(2) yes
    O1 O3 O4 1_655 . 4_655 59.220(15) yes
    O1 O3 O5 1_655 . 1_545 68.675(16) yes
    O1 O3 O5 1_655 . 2_745 60.225(16) yes
    O1 O3 O1 4_655 . 1_655 89.077(15) yes
    O1 O3 O2 4_655 . 2_645 151.77(2) yes
    O1 O3 O4 4_655 . 2_645 128.13(2) yes
    O1 O3 O4 4_655 . 4_655 60.873(13) yes
    O1 O3 O5 4_655 . 1_545 147.377(19) yes
    O1 O3 O5 4_655 . 2_745 59.552(14) yes
    O2 O3 O4 2_645 . 2_645 62.501(14) yes
    O2 O3 O4 2_645 . 4_655 147.11(2) yes
    O2 O3 O5 2_645 . 1_545 60.256(14) yes
    O2 O3 O5 2_645 . 2_745 105.406(17) yes
    O4 O3 O4 2_645 . 4_655 102.731(16) yes
    O4 O3 O5 2_645 . 1_545 59.885(15) yes
    O4 O3 O5 2_645 . 2_745 166.447(17) yes
    O4 O3 O4 4_655 . 2_645 102.731(16) yes
    O4 O3 O5 4_655 . 1_545 86.850(16) yes
    O4 O3 O5 4_655 . 2_745 90.801(16) yes
    O5 O3 O5 1_545 . 2_745 121.07(2) yes
    O5 O3 O5 2_745 . 1_545 121.07(2) yes
    Na O4 Na 2_645 . 4_564 104.15(2) yes
    Na O4 Ta 2_645 . 2_645 100.70(2) yes
    Na O4 Ge 2_645 . . 116.593(19) yes
    Na O4 O1 2_645 . . 97.525(17) yes
    Na O4 O1 2_645 . 4_554 97.99(2) yes
    Na O4 O2 2_645 . . 84.793(16) yes
    Na O4 O2 2_645 . 2_645 55.895(16) yes
    Na O4 O3 2_645 . 2_655 137.49(2) yes
    Na O4 O3 2_645 . 4_454 145.21(2) yes
    Na O4 O5 2_645 . 2_645 117.010(18) yes
    Na O4 Na 4_564 . 2_645 104.15(2) yes
    Na O4 Ta 4_564 . 2_645 91.518(18) yes
    Na O4 Ge 4_564 . . 110.504(19) yes
    Na O4 O1 4_564 . . 134.164(17) yes
    Na O4 O1 4_564 . 4_554 49.643(16) yes
    Na O4 O2 4_564 . . 110.804(18) yes
    Na O4 O2 4_564 . 2_645 101.18(2) yes
    Na O4 O3 4_564 . 2_655 76.598(16) yes
    Na O4 O3 4_564 . 4_454 82.615(15) yes
    Na O4 O5 4_564 . 2_645 134.996(18) yes
    Ta O4 Ge 2_645 . . 128.65(3) yes
    Ta O4 O1 2_645 . . 44.477(11) yes
    Ta O4 O1 2_645 . 4_554 43.510(12) yes
    Ta O4 O2 2_645 . . 155.13(2) yes
    Ta O4 O2 2_645 . 2_645 44.809(11) yes
    Ta O4 O3 2_645 . 2_655 121.802(18) yes
    Ta O4 O3 2_645 . 4_454 44.572(11) yes
    Ta O4 O5 2_645 . 2_645 97.670(19) yes
    Ge O4 O1 . . . 94.31(2) yes
    Ge O4 O1 . . 4_554 144.624(19) yes
    Ge O4 O2 . . . 33.807(11) yes
    Ge O4 O2 . . 2_645 148.15(2) yes
    Ge O4 O3 . . 2_655 35.363(11) yes
    Ge O4 O3 . . 4_454 91.49(2) yes
    Ge O4 O5 . . 2_645 34.887(12) yes
    O1 O4 O1 . . 4_554 87.987(15) yes
    O1 O4 O2 . . . 110.99(2) yes
    O1 O4 O2 . . 2_645 59.699(14) yes
    O1 O4 O3 . . 2_655 112.26(2) yes
    O1 O4 O3 . . 4_454 58.039(12) yes
    O1 O4 O5 . . 2_645 59.431(14) yes
    O1 O4 O1 4_554 . . 87.987(15) yes
    O1 O4 O2 4_554 . . 160.39(2) yes
    O1 O4 O2 4_554 . 2_645 59.052(14) yes
    O1 O4 O3 4_554 . 2_655 112.153(15) yes
    O1 O4 O3 4_554 . 4_454 60.141(14) yes
    O1 O4 O5 4_554 . 2_645 133.534(18) yes
    O2 O4 O2 . . 2_645 134.516(16) yes
    O2 O4 O3 . . 2_655 57.009(13) yes
    O2 O4 O3 . . 4_454 125.29(2) yes
    O2 O4 O5 . . 2_645 58.935(15) yes
    O2 O4 O2 2_645 . . 134.516(16) yes
    O2 O4 O3 2_645 . 2_655 166.606(17) yes
    O2 O4 O3 2_645 . 4_454 89.360(15) yes
    O2 O4 O5 2_645 . 2_645 116.208(18) yes
    O3 O4 O3 2_655 . 4_454 77.269(15) yes
    O3 O4 O5 2_655 . 2_645 61.136(15) yes
    O3 O4 O3 4_454 . 2_655 77.269(15) yes
    O3 O4 O5 4_454 . 2_645 74.101(17) yes
    Na O5 Na 1_655 . 3_675 101.81(2) yes
    Na O5 Ta 1_655 . 4_564 100.27(2) yes
    Na O5 Ge 1_655 . 2_655 117.456(19) yes
    Na O5 O1 1_655 . 3_665 95.95(2) yes
    Na O5 O1 1_655 . 2_655 98.521(18) yes
    Na O5 O2 1_655 . 2_655 137.11(2) yes
    Na O5 O2 1_655 . 4_564 144.56(2) yes
    Na O5 O3 1_655 . 1_565 85.490(16) yes
    Na O5 O3 1_655 . 2_755 55.504(16) yes
    Na O5 O4 1_655 . 2_655 119.326(18) yes
    Na O5 Na 3_675 . 1_655 101.81(2) yes
    Na O5 Ta 3_675 . 4_564 94.795(18) yes
    Na O5 Ge 3_675 . 2_655 110.087(19) yes
    Na O5 O1 3_675 . 3_665 50.857(16) yes
    Na O5 O1 3_675 . 2_655 135.776(18) yes
    Na O5 O2 3_675 . 2_655 76.118(16) yes
    Na O5 O2 3_675 . 4_564 83.448(15) yes
    Na O5 O3 3_675 . 1_565 110.093(19) yes
    Na O5 O3 3_675 . 2_755 101.99(2) yes
    Na O5 O4 3_675 . 2_655 134.574(18) yes
    Ta O5 Ge 4_564 . 2_655 127.68(3) yes
    Ta O5 O1 4_564 . 3_665 45.671(12) yes
    Ta O5 O1 4_564 . 2_655 42.760(10) yes
    Ta O5 O2 4_564 . 2_655 122.614(18) yes
    Ta O5 O2 4_564 . 4_564 44.315(11) yes
    Ta O5 O3 4_564 . 1_565 152.85(2) yes
    Ta O5 O3 4_564 . 2_755 44.769(11) yes
    Ta O5 O4 4_564 . 2_655 95.912(18) yes
    Ge O5 O1 2_655 . 3_665 145.594(19) yes
    Ge O5 O1 2_655 . 2_655 94.16(2) yes
    Ge O5 O2 2_655 . 2_655 35.560(11) yes
    Ge O5 O2 2_655 . 4_564 92.45(2) yes
    Ge O5 O3 2_655 . 1_565 33.581(11) yes
    Ge O5 O3 2_655 . 2_755 147.86(2) yes
    Ge O5 O4 2_655 . 2_655 34.856(12) yes
    O1 O5 O1 3_665 . 2_655 88.431(15) yes
    O1 O5 O2 3_665 . 2_655 112.922(15) yes
    O1 O5 O2 3_665 . 4_564 60.104(14) yes
    O1 O5 O3 3_665 . 1_565 160.83(2) yes
    O1 O5 O3 3_665 . 2_755 58.833(14) yes
    O1 O5 O4 3_665 . 2_655 133.697(18) yes
    O1 O5 O1 2_655 . 3_665 88.431(15) yes
    O1 O5 O2 2_655 . 2_655 112.69(2) yes
    O1 O5 O2 2_655 . 4_564 58.337(12) yes
    O1 O5 O3 2_655 . 1_565 110.313(19) yes
    O1 O5 O3 2_655 . 2_755 59.815(14) yes
    O1 O5 O4 2_655 . 2_655 59.308(14) yes
    O2 O5 O2 2_655 . 4_564 78.305(15) yes
    O2 O5 O3 2_655 . 1_565 56.984(13) yes
    O2 O5 O3 2_655 . 2_755 167.348(17) yes
    O2 O5 O4 2_655 . 2_655 61.027(15) yes
    O2 O5 O2 4_564 . 2_655 78.305(15) yes
    O2 O5 O3 4_564 . 1_565 126.03(2) yes
    O2 O5 O3 4_564 . 2_755 89.062(15) yes
    O2 O5 O4 4_564 . 2_655 74.272(17) yes
    O3 O5 O3 1_565 . 2_755 133.870(15) yes
    O3 O5 O4 1_565 . 2_655 58.979(15) yes
    O3 O5 O3 2_755 . 1_565 133.870(15) yes
    O3 O5 O4 2_755 . 2_655 116.386(18) yes
data_2
_chemical_name_systematic
; ?
;
_chemical_name_common     ?
_chemical_formula_moiety     ?
_chemical_formula_sum     'Ge1 Na1 O5 Ta1'
_chemical_formula_structural     ?
_chemical_formula_analytical     ?
_chemical_formula_iupac     ?
_chemical_formula_weight     356.5
_chemical_melting_point     ?
_symmetry_cell_setting     monoclinic
_symmetry_space_group_name_H-M     'C 1 2/c 1'
_symmetry_space_group_name_Hall     '-C 2yc'
loop_
    _symmetry_equiv_pos_site_id
    _symmetry_equiv_pos_as_xyz
    1 x,y,z
    2 -x,y,1/2-z
    3 -x,-y,-z
    4 x,-y,1/2+z
    5 1/2+x,1/2+y,z
    6 1/2-x,1/2+y,1/2-z
    7 1/2-x,1/2-y,-z
    8 1/2+x,1/2-y,1/2+z
_cell_length_a     6.8540(10)
_cell_length_b     8.9330(10)
_cell_length_c     7.4180(10)
_cell_angle_alpha     90
_cell_angle_beta     114.858(2)
_cell_angle_gamma     90
_cell_volume     412.10(9)
_cell_formula_units_Z     4
_cell_measurement_reflns_used     ?
_cell_measurement_theta_min     ?
_cell_measurement_theta_max     ?
_cell_measurement_temperature     295
_cell_special_details
; ?
;
_exptl_crystal_description     Tabular
_exptl_crystal_colour     colourless
_exptl_crystal_size_max     0.1
_exptl_crystal_size_mid     0.09
_exptl_crystal_size_min     0.045
_exptl_crystal_size_rad     ?
_exptl_crystal_density_diffrn     5.7445
_exptl_crystal_density_meas     ?
_exptl_crystal_density_method     ?
_exptl_crystal_F_000     624
_exptl_absorpt_coefficient_mu     6.954
_exptl_absorpt_correction_type     None
_exptl_absorpt_correction_T_min     ?
_exptl_absorpt_correction_T_max     ?
_exptl_special_details     ?
_diffrn_ambient_temperature     295
_diffrn_radiation_type     'synchrotron'
_diffrn_radiation_wavelength     0.39184
_diffrn_radiation_source     ?
_diffrn_radiation_monochromator     ?
_diffrn_measurement_device_type     'beamline F1 at Hasylab'
_diffrn_measurement_method     'φ-scan'
_diffrn_detector_area_resol_mean     ?
_diffrn_reflns_number     95651
_diffrn_reflns_av_R_equivalents     0.0483
_diffrn_reflns_av_sigmaI/netI     0.0263
_diffrn_reflns_theta_min     2.26
_diffrn_reflns_theta_max     53.34
_diffrn_reflns_theta_full     53.34
_diffrn_measured_fraction_theta_max     ?
_diffrn_measured_fraction_theta_full     0.96
_diffrn_reflns_limit_h_min     -28
_diffrn_reflns_limit_h_max     28
_diffrn_reflns_limit_k_min     -35
_diffrn_reflns_limit_k_max     29
_diffrn_reflns_limit_l_min     -29
_diffrn_reflns_limit_l_max     26
_diffrn_reflns_reduction_process     ?
_diffrn_standards_number     ?
_diffrn_standards_interval_count     ?
_diffrn_standards_interval_time     ?
_diffrn_standards_decay_%     ?
_refine_special_details
; ?
;
_reflns_number_total     14190
_reflns_number_gt     11959
_reflns_threshold_expression     'I>3σ(I)'
_refine_ls_structure_factor_coef     Fsqd
_refine_ls_R_factor_all     0.0257
_refine_ls_R_factor_gt     0.0199
_refine_ls_wR_factor_gt     0.0610
_refine_ls_wR_factor_ref     0.0662
_refine_ls_goodness_of_fit_ref     1.02
_refine_ls_restrained_S_all     ?
_refine_ls_number_reflns     14190
_refine_ls_number_parameters     54
_refine_ls_number_restraints     ?
_refine_ls_number_constraints     ?
_refine_ls_hydrogen_treatment     ?
_refine_ls_weighting_scheme     sigma
_refine_ls_weighting_details     'w=1/(σ²(I)+0.0016I²)'
_refine_ls_shift/su_max     0.0006
_refine_ls_shift/su_mean     0.0001
_refine_diff_density_max     2.59
_refine_diff_density_min     -2.42
_refine_ls_extinction_method
                        'B-C type 1 Gaussian isotropic (Becker & Coppens, 1974)'
_refine_ls_extinction_coef     0.00728(19)
loop_
    _atom_type_symbol
    _atom_type_scat_dispersion_real
    _atom_type_scat_dispersion_imag
    _atom_type_scat_source
    Na 0.009 0.007 'International Tables Vol C Tables  4.2.6.8 and 6.1.1.4'
    Ta -0.553 2.507 'International Tables Vol C Tables  4.2.6.8 and 6.1.1.4'
    Ge 0.275 0.650 'International Tables Vol C Tables  4.2.6.8 and 6.1.1.4'
    O 0.002 0.002 'International Tables Vol C Tables  4.2.6.8 and 6.1.1.4'
_computing_data_collection     ?
_computing_cell_refinement     ?
_computing_data_reduction     ?
_computing_structure_solution     ?
_computing_structure_refinement     '(Jana2000; Petricek and Dusek, 2000)'
_computing_molecular_graphics     ?
_computing_publication_material     '(Jana2000; Petricek and Dusek, 2000)'
loop_
    _atom_site_type_symbol
    _atom_site_label
    _atom_site_fract_x
    _atom_site_fract_y
    _atom_site_fract_z
    _atom_site_U_iso_or_equiv
    _atom_site_adp_type
    _atom_site_calc_flag
    _atom_site_refinement_flags
    _atom_site_occupancy
    _atom_site_disorder_assembly
    _atom_site_disorder_group
    Na Na 0 0.32594(11) 0.75 0.0200(2) Uani d . 1 . .
    Ta Ta 0 0 0 0.006843(5) Uani d . 1 . .
    Ge Ge 0 0.317582(8) 0.25 0.006317(8) Uani d . 1 . .
    O O1 0 0.06634(6) 0.75 0.00941(7) Uani d . 1 . .
    O O2 0.19575(6) 0.43833(5) 0.41118(6) 0.01141(6) Uani d . 1 . .
    O O3 0.09772(6) 0.20534(4) 0.11237(6) 0.01002(6) Uani d . 1 . .
loop_
    _atom_site_aniso_label
    _atom_site_aniso_U_11
    _atom_site_aniso_U_22
    _atom_site_aniso_U_33
    _atom_site_aniso_U_12
    _atom_site_aniso_U_13
    _atom_site_aniso_U_23
    _atom_site_aniso_type_symbol
    Na 0.0153(3) 0.0127(3) 0.0282(4) 0 0.0053(3) 0 Na
    Ta 0.006618(6) 0.006617(7) 0.006871(7) 0.000740(2) 0.002422(4) -0.000577(3)
                                                                              Ta
    Ge 0.006038(10) 0.005849(11) 0.006682(12) 0 0.002299(8) 0 Ge
    O1 0.01312(12) 0.00965(9) 0.00612(7) 0 0.00471(7) 0 O
    O2 0.00816(6) 0.01219(9) 0.01282(9) -0.00334(6) 0.00336(6) -0.00369(8) O
    O3 0.01225(8) 0.00757(6) 0.01229(8) -0.00119(6) 0.00715(7) -0.00271(6) O
loop_
    _geom_bond_atom_site_label_1
    _geom_bond_atom_site_label_2
    _geom_bond_site_symmetry_1
    _geom_bond_site_symmetry_2
    _geom_bond_distance
    _geom_bond_publ_flag
    Na O1 . . 2.3189(11) yes
    Na O2 . 3_566 2.5130(9) yes
    Na O2 . 4_565 2.5130(9) yes
    Na O3 . 1_556 2.7058(6) yes
    Na O3 . 7_556 2.5211(4) yes
    Na O3 . 2_555 2.7057(6) yes
    Na O3 . 8_455 2.5211(4) yes
    Ta O1 . 1_554 1.9469(2) yes
    Ta O1 . 3_556 1.9469(2) yes
    Ta O2 . 6_545 1.9827(4) yes
    Ta O2 . 8_454 1.9827(4) yes
    Ta O3 . . 2.0096(3) yes
    Ta O3 . 3_555 2.0096(3) yes
    Ge O2 . . 1.7448(4) yes
    Ge O2 . 2_555 1.7448(4) yes
    Ge O3 . . 1.7525(5) yes
    Ge O3 . 2_555 1.7525(5) yes
    O1 O2 . 5_445 2.7508(4) yes
    O1 O2 . 7_556 2.8064(5) yes
    O1 O2 . 6_546 2.7508(4) yes
    O1 O2 . 8_455 2.8064(5) yes
    O1 O3 . 1_556 2.7753(5) yes
    O1 O3 . 3_556 2.8206(6) yes
    O1 O3 . 2_555 2.7753(5) yes
    O1 O3 . 4_555 2.8206(6) yes
    O2 O2 . 2_555 2.7429(4) yes
    O2 O3 . . 2.9059(6) yes
    O2 O3 . 2_555 2.8483(6) yes
    O2 O3 . 6_555 2.8162(6) yes
    O2 O3 . 8_555 2.8298(5) yes
    O3 O3 . 2_555 2.8746(7) yes
loop_
    _geom_angle_atom_site_label_1
    _geom_angle_atom_site_label_2
    _geom_angle_atom_site_label_3
    _geom_angle_site_symmetry_1
    _geom_angle_site_symmetry_2
    _geom_angle_site_symmetry_3
    _geom_angle
    _geom_angle_publ_flag
    O1 Na O2 . . 3_566 146.925(14) yes
    O1 Na O2 . . 4_565 146.925(14) yes
    O1 Na O3 . . 1_556 66.54(2) yes
    O1 Na O3 . . 7_556 83.64(2) yes
    O1 Na O3 . . 2_555 66.54(2) yes
    O1 Na O3 . . 8_455 83.64(2) yes
    O2 Na O2 3_566 . 4_565 66.15(3) yes
    O2 Na O3 3_566 . 1_556 131.76(2) yes
    O2 Na O3 3_566 . 7_556 124.04(3) yes
    O2 Na O3 3_566 . 2_555 90.075(15) yes
    O2 Na O3 3_566 . 8_455 68.032(16) yes
    O2 Na O2 4_565 . 3_566 66.15(3) yes
    O2 Na O3 4_565 . 1_556 90.075(15) yes
    O2 Na O3 4_565 . 7_556 68.032(16) yes
    O2 Na O3 4_565 . 2_555 131.76(2) yes
    O2 Na O3 4_565 . 8_455 124.04(3) yes
    O3 Na O3 1_556 . 7_556 77.393(16) yes
    O3 Na O3 1_556 . 2_555 133.07(4) yes
    O3 Na O3 1_556 . 8_455 97.472(18) yes
    O3 Na O3 7_556 . 1_556 77.393(16) yes
    O3 Na O3 7_556 . 2_555 97.472(18) yes
    O3 Na O3 7_556 . 8_455 167.28(4) yes
    O3 Na O3 2_555 . 1_556 133.07(4) yes
    O3 Na O3 2_555 . 7_556 97.472(18) yes
    O3 Na O3 2_555 . 8_455 77.393(16) yes
    O3 Na O3 8_455 . 1_556 97.472(18) yes
    O3 Na O3 8_455 . 7_556 167.28(4) yes
    O3 Na O3 8_455 . 2_555 77.393(16) yes
    O1 Ta O1 1_554 . 3_556 180 yes
    O1 Ta O2 1_554 . 6_545 88.853(15) yes
    O1 Ta O2 1_554 . 8_454 91.147(15) yes
    O1 Ta O3 1_554 . . 89.072(19) yes
    O1 Ta O3 1_554 . 3_555 90.928(19) yes
    O1 Ta O1 3_556 . 1_554 180 yes
    O1 Ta O2 3_556 . 6_545 91.147(15) yes
    O1 Ta O2 3_556 . 8_454 88.853(15) yes
    O1 Ta O3 3_556 . . 90.928(19) yes
    O1 Ta O3 3_556 . 3_555 89.072(19) yes
    O2 Ta O2 6_545 . 8_454 180 yes
    O2 Ta O3 6_545 . . 89.724(17) yes
    O2 Ta O3 6_545 . 3_555 90.276(17) yes
    O2 Ta O2 8_454 . 6_545 180 yes
    O2 Ta O3 8_454 . . 90.276(17) yes
    O2 Ta O3 8_454 . 3_555 89.724(17) yes
    O3 Ta O3 . . 3_555 180 yes
    O3 Ta O3 3_555 . . 180 yes
    O2 Ge O2 . . 2_555 103.630(18) yes
    O2 Ge O3 . . . 112.38(2) yes
    O2 Ge O3 . . 2_555 109.06(2) yes
    O2 Ge O2 2_555 . . 103.630(18) yes
    O2 Ge O3 2_555 . . 109.06(2) yes
    O2 Ge O3 2_555 . 2_555 112.38(2) yes
    O3 Ge O3 . . 2_555 110.199(19) yes
    O3 Ge O3 2_555 . . 110.199(19) yes
    Na O1 Ta . . 1_556 107.722(14) yes
    Na O1 Ta . . 2_555 107.722(14) yes
    Na O1 O2 . . 5_445 114.564(13) yes
    Na O1 O2 . . 7_556 90.852(13) yes
    Na O1 O2 . . 6_546 114.564(13) yes
    Na O1 O2 . . 8_455 90.852(13) yes
    Na O1 O3 . . 1_556 63.424(12) yes
    Na O1 O3 . . 3_556 149.364(11) yes
    Na O1 O3 . . 2_555 63.424(12) yes
    Na O1 O3 . . 4_555 149.364(11) yes
    Ta O1 Ta 1_556 . 2_555 144.56(3) yes
    Ta O1 O2 1_556 . 5_445 116.119(18) yes
    Ta O1 O2 1_556 . 7_556 134.332(12) yes
    Ta O1 O2 1_556 . 6_546 46.106(11) yes
    Ta O1 O2 1_556 . 8_455 44.938(7) yes
    Ta O1 O3 1_556 . 1_556 46.387(9) yes
    Ta O1 O3 1_556 . 3_556 45.429(12) yes
    Ta O1 O3 1_556 . 2_555 164.187(16) yes
    Ta O1 O3 1_556 . 4_555 100.25(2) yes
    Ta O1 Ta 2_555 . 1_556 144.56(3) yes
    Ta O1 O2 2_555 . 5_445 46.106(11) yes
    Ta O1 O2 2_555 . 7_556 44.938(7) yes
    Ta O1 O2 2_555 . 6_546 116.119(18) yes
    Ta O1 O2 2_555 . 8_455 134.332(12) yes
    Ta O1 O3 2_555 . 1_556 164.187(16) yes
    Ta O1 O3 2_555 . 3_556 100.25(2) yes
    Ta O1 O3 2_555 . 2_555 46.387(9) yes
    Ta O1 O3 2_555 . 4_555 45.429(12) yes
    O2 O1 O2 5_445 . 7_556 91.044(14) yes
    O2 O1 O2 5_445 . 6_546 130.87(2) yes
    O2 O1 O2 5_445 . 8_455 88.247(14) yes
    O2 O1 O3 5_445 . 1_556 148.491(14) yes
    O2 O1 O3 5_445 . 3_556 76.638(16) yes
    O2 O1 O3 5_445 . 2_555 61.276(12) yes
    O2 O1 O3 5_445 . 4_555 61.036(14) yes
    O2 O1 O2 7_556 . 5_445 91.044(14) yes
    O2 O1 O2 7_556 . 6_546 88.247(14) yes
    O2 O1 O2 7_556 . 8_455 178.30(2) yes
    O2 O1 O3 7_556 . 1_556 119.953(14) yes
    O2 O1 O3 7_556 . 3_556 118.26(2) yes
    O2 O1 O3 7_556 . 2_555 60.923(12) yes
    O2 O1 O3 7_556 . 4_555 60.064(14) yes
    O2 O1 O2 6_546 . 5_445 130.87(2) yes
    O2 O1 O2 6_546 . 7_556 88.247(14) yes
    O2 O1 O2 6_546 . 8_455 91.044(14) yes
    O2 O1 O3 6_546 . 1_556 61.276(12) yes
    O2 O1 O3 6_546 . 3_556 61.036(14) yes
    O2 O1 O3 6_546 . 2_555 148.490(14) yes
    O2 O1 O3 6_546 . 4_555 76.638(16) yes
    O2 O1 O2 8_455 . 5_445 88.247(14) yes
    O2 O1 O2 8_455 . 7_556 178.30(2) yes
    O2 O1 O2 8_455 . 6_546 91.044(14) yes
    O2 O1 O3 8_455 . 1_556 60.923(12) yes
    O2 O1 O3 8_455 . 3_556 60.064(14) yes
    O2 O1 O3 8_455 . 2_555 119.953(14) yes
    O2 O1 O3 8_455 . 4_555 118.26(2) yes
    O3 O1 O3 1_556 . 3_556 91.816(13) yes
    O3 O1 O3 1_556 . 2_555 126.85(2) yes
    O3 O1 O3 1_556 . 4_555 137.578(15) yes
    O3 O1 O3 3_556 . 1_556 91.816(13) yes
    O3 O1 O3 3_556 . 2_555 137.578(15) yes
    O3 O1 O3 3_556 . 4_555 61.271(17) yes
    O3 O1 O3 2_555 . 1_556 126.85(2) yes
    O3 O1 O3 2_555 . 3_556 137.578(15) yes
    O3 O1 O3 2_555 . 4_555 91.816(13) yes
    O3 O1 O3 4_555 . 1_556 137.578(15) yes
    O3 O1 O3 4_555 . 3_556 61.271(17) yes
    O3 O1 O3 4_555 . 2_555 91.816(13) yes
    Na O2 Ta 3_566 . 6_555 101.65(2) yes
    Na O2 Ge 3_566 . . 95.110(18) yes
    Na O2 O1 3_566 . 5_555 97.72(2) yes
    Na O2 O1 3_566 . 7_556 98.829(18) yes
    Na O2 O2 3_566 . 2_555 56.925(16) yes
    Na O2 O3 3_566 . . 109.346(18) yes
    Na O2 O3 3_566 . 2_555 111.170(17) yes
    Na O2 O3 3_566 . 6_555 56.121(15) yes
    Na O2 O3 3_566 . 8_555 146.89(2) yes
    Ta O2 Ge 6_555 . . 142.93(3) yes
    Ta O2 O1 6_555 . 5_555 45.041(7) yes
    Ta O2 O1 6_555 . 7_556 43.915(11) yes
    Ta O2 O2 6_555 . 2_555 142.80(3) yes
    Ta O2 O3 6_555 . . 109.03(2) yes
    Ta O2 O3 6_555 . 2_555 147.18(2) yes
    Ta O2 O3 6_555 . 6_555 45.526(12) yes
    Ta O2 O3 6_555 . 8_555 45.246(11) yes
    Ge O2 O1 . . 5_555 162.23(3) yes
    Ge O2 O1 . . 7_556 101.18(2) yes
    Ge O2 O2 . . 2_555 38.185(11) yes
    Ge O2 O3 . . . 33.892(13) yes
    Ge O2 O3 . . 2_555 35.558(13) yes
    Ge O2 O3 . . 6_555 137.97(2) yes
    Ge O2 O3 . . 8_555 112.26(2) yes
    O1 O2 O1 5_555 . 7_556 88.956(11) yes
    O1 O2 O2 5_555 . 2_555 152.20(2) yes
    O1 O2 O3 5_555 . . 146.938(18) yes
    O1 O2 O3 5_555 . 2_555 127.18(2) yes
    O1 O2 O3 5_555 . 6_555 59.790(13) yes
    O1 O2 O3 5_555 . 8_555 60.699(13) yes
    O1 O2 O1 7_556 . 5_555 88.956(11) yes
    O1 O2 O2 7_556 . 2_555 104.976(19) yes
    O1 O2 O3 7_556 . . 68.860(17) yes
    O1 O2 O3 7_556 . 2_555 126.52(2) yes
    O1 O2 O3 7_556 . 6_555 60.217(17) yes
    O1 O2 O3 7_556 . 8_555 58.995(14) yes
    O2 O2 O3 2_555 . . 60.479(14) yes
    O2 O2 O3 2_555 . 2_555 62.595(14) yes
    O2 O2 O3 2_555 . 6_555 106.199(18) yes
    O2 O2 O3 2_555 . 8_555 146.99(2) yes
    O3 O2 O3 . . 2_555 59.932(16) yes
    O3 O2 O3 . . 6_555 121.36(2) yes
    O3 O2 O3 . . 8_555 86.510(16) yes
    O3 O2 O3 2_555 . . 59.932(16) yes
    O3 O2 O3 2_555 . 6_555 167.287(17) yes
    O3 O2 O3 2_555 . 8_555 101.935(17) yes
    O3 O2 O3 6_555 . . 121.36(2) yes
    O3 O2 O3 6_555 . 2_555 167.287(17) yes
    O3 O2 O3 6_555 . 8_555 90.772(15) yes
    O3 O2 O3 8_555 . . 86.510(16) yes
    O3 O2 O3 8_555 . 2_555 101.935(17) yes
    O3 O2 O3 8_555 . 6_555 90.772(15) yes
    Na O3 Na 1_554 . 7_556 102.607(19) yes
    Na O3 Ta 1_554 . . 92.94(2) yes
    Na O3 Ge 1_554 . . 110.81(2) yes
    Na O3 O1 1_554 . 1_554 50.04(2) yes
    Na O3 O1 1_554 . 3_556 134.82(2) yes
    Na O3 O2 1_554 . . 110.73(2) yes
    Na O3 O2 1_554 . 2_555 76.976(18) yes
    Na O3 O2 1_554 . 6_545 101.34(2) yes
    Na O3 O2 1_554 . 8_454 82.941(17) yes
    Na O3 O3 1_554 . 2_555 135.319(18) yes
    Na O3 Na 7_556 . 1_554 102.607(19) yes
    Na O3 Ta 7_556 . . 100.60(3) yes
    Na O3 Ge 7_556 . . 116.63(2) yes
    Na O3 O1 7_556 . 1_554 96.905(19) yes
    Na O3 O1 7_556 . 3_556 98.27(2) yes
    Na O3 O2 7_556 . . 84.70(2) yes
    Na O3 O2 7_556 . 2_555 136.86(3) yes
    Na O3 O2 7_556 . 6_545 55.85(2) yes
    Na O3 O2 7_556 . 8_454 145.07(3) yes
    Na O3 O3 7_556 . 2_555 117.982(15) yes
    Ta O3 Ge . . . 128.43(3) yes
    Ta O3 O1 . . 1_554 44.541(12) yes
    Ta O3 O1 . . 3_556 43.642(9) yes
    Ta O3 O2 . . . 154.16(2) yes
    Ta O3 O2 . . 2_555 122.541(18) yes
    Ta O3 O2 . . 6_545 44.750(10) yes
    Ta O3 O2 . . 8_454 44.478(11) yes
    Ta O3 O3 . . 2_555 96.953(18) yes
    Ge O3 O1 . . 1_554 145.540(18) yes
    Ge O3 O1 . . 3_556 94.26(2) yes
    Ge O3 O2 . . . 33.724(10) yes
    Ge O3 O2 . . 2_555 35.379(12) yes
    Ge O3 O2 . . 6_545 147.76(2) yes
    Ge O3 O2 . . 8_454 92.35(2) yes
    Ge O3 O3 . . 2_555 34.901(12) yes
    O1 O3 O1 1_554 . 3_556 88.184(14) yes
    O1 O3 O2 1_554 . . 160.65(2) yes
    O1 O3 O2 1_554 . 2_555 113.008(15) yes
    O1 O3 O2 1_554 . 6_545 58.934(14) yes
    O1 O3 O2 1_554 . 8_454 60.082(13) yes
    O1 O3 O3 1_554 . 2_555 133.886(16) yes
    O1 O3 O1 3_556 . 1_554 88.184(14) yes
    O1 O3 O2 3_556 . . 110.739(19) yes
    O1 O3 O2 3_556 . 2_555 112.45(2) yes
    O1 O3 O2 3_556 . 6_545 59.719(13) yes
    O1 O3 O2 3_556 . 8_454 58.265(12) yes
    O1 O3 O3 3_556 . 2_555 59.364(13) yes
    O2 O3 O2 . . 2_555 56.926(13) yes
    O2 O3 O2 . . 6_545 133.854(16) yes
    O2 O3 O2 . . 8_454 126.07(2) yes
    O2 O3 O3 . . 2_555 59.039(15) yes
    O2 O3 O2 2_555 . . 56.926(13) yes
    O2 O3 O2 2_555 . 6_545 167.287(17) yes
    O2 O3 O2 2_555 . 8_454 78.065(15) yes
    O2 O3 O3 2_555 . 2_555 61.029(16) yes
    O2 O3 O2 6_545 . . 133.854(16) yes
    O2 O3 O2 6_545 . 2_555 167.287(17) yes
    O2 O3 O2 6_545 . 8_454 89.228(15) yes
    O2 O3 O3 6_545 . 2_555 116.137(18) yes
    O2 O3 O2 8_454 . . 126.07(2) yes
    O2 O3 O2 8_454 . 2_555 78.065(15) yes
    O2 O3 O2 8_454 . 6_545 89.228(15) yes
    O2 O3 O3 8_454 . 2_555 74.547(17) yes
